#------------------------------------------------------------------------------
#$Date: 2016-03-22 11:19:20 +0200 (Tue, 22 Mar 2016) $
#$Revision: 178894 $
#$URL: svn://www.crystallography.net/cod/cif/4/11/23/4112389.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4112389
loop_
_publ_author_name
'Li-Ming Wu'
'Dong-Kyun Seo'
_publ_section_title
;
 Mn14Al56+xGe3-x (x= 0-0.6): A New Intermetallic Phase Containing
 Unprecedented "Half-Broken" Mackay Icosahedra as Building Units
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              4398
_journal_page_last               4403
_journal_paper_doi               10.1021/ja039154f
_journal_volume                  126
_journal_year                    2004
_chemical_formula_sum            'Al56 Ge3 Mn14'
_chemical_formula_weight         2497.81
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           147
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-P 3'
_symmetry_space_group_name_H-M   'P -3'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.000(4)
_cell_angle_beta                 90.000(4)
_cell_angle_gamma                120.000(4)
_cell_formula_units_Z            1
_cell_length_a                   11.098(2)
_cell_length_b                   11.098(2)
_cell_length_c                   10.3496(19)
_cell_measurement_temperature    298(2)
_cell_volume                     1103.9(3)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0618
_diffrn_reflns_av_sigmaI/netI    0.0427
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            13099
_diffrn_reflns_theta_full        29.99
_diffrn_reflns_theta_max         29.99
_diffrn_reflns_theta_min         1.97
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    6.997
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'SADABS (Sheldrick, 1996)'
_exptl_crystal_colour            Silvery
_exptl_crystal_density_diffrn    3.757
_exptl_crystal_description       Block
_exptl_crystal_F_000             1174
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.04
_refine_diff_density_max         0.873
_refine_diff_density_min         -1.182
_refine_diff_density_rms         0.193
_refine_ls_extinction_coef       0.00075(14)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.072
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     112
_refine_ls_number_reflns         2165
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.072
_refine_ls_R_factor_all          0.0465
_refine_ls_R_factor_gt           0.0431
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0000P)²+9.8606P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0848
_refine_ls_wR_factor_ref         0.0865
_reflns_number_gt                2048
_reflns_number_total             2165
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja039154fsi20031213_050058.cif
_cod_data_source_block           w274
_cod_database_code               4112389
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Mn1 Mn 0.3333 0.6667 0.44543(10) 0.0043(2) Uani 1 3 d S
Mn2 Mn 0.36088(6) 0.42294(6) 0.07157(6) 0.00497(14) Uani 1 1 d .
Mn3 Mn 0.25794(6) 0.04830(6) 0.33116(6) 0.00514(14) Uani 1 1 d .
Ge1 Ge 0.0000 0.0000 0.0000 0.0072(2) Uani 1 6 d S
Ge2 Ge 0.3333 0.6667 0.72050(8) 0.01115(18) Uani 1 3 d S
Al1 Al 0.0000 0.0000 0.7452(2) 0.0094(4) Uani 1 3 d S
Al2 Al 0.26218(14) 0.13084(14) 0.08429(13) 0.0093(3) Uani 1 1 d .
Al3 Al 0.49290(14) 0.11437(14) 0.43643(13) 0.0088(3) Uani 1 1 d .
Al4 Al 0.13824(14) 0.41657(14) 0.45323(14) 0.0105(3) Uani 1 1 d .
Al5 Al 0.16740(15) 0.62423(15) 0.27359(13) 0.0116(3) Uani 1 1 d .
Al6 Al 0.19202(13) 0.51319(14) 0.01594(13) 0.0082(3) Uani 1 1 d .
Al7 Al 0.44767(14) 0.06341(14) 0.17098(13) 0.0091(3) Uani 1 1 d .
Al8 Al 0.40738(13) 0.30495(14) 0.26899(13) 0.0078(2) Uani 1 1 d .
Al9 Al 0.14556(14) 0.30021(14) 0.18802(13) 0.0094(3) Uani 1 1 d .
Al10 Al 0.16646(14) 0.19503(14) 0.42175(12) 0.0083(3) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Al5 Mn1 Al5 72.37(6) . 3_565
Al5 Mn1 Al5 72.37(6) . 2_665
Al5 Mn1 Al5 72.37(6) 3_565 2_665
Al5 Mn1 Al4 72.86(5) . 3_565
Al5 Mn1 Al4 70.16(5) 3_565 3_565
Al5 Mn1 Al4 134.77(6) 2_665 3_565
Al5 Mn1 Al4 70.16(5) . .
Al5 Mn1 Al4 134.77(6) 3_565 .
Al5 Mn1 Al4 72.86(5) 2_665 .
Al4 Mn1 Al4 119.899(5) 3_565 .
Al5 Mn1 Al4 134.77(6) . 2_665
Al5 Mn1 Al4 72.86(5) 3_565 2_665
Al5 Mn1 Al4 70.16(5) 2_665 2_665
Al4 Mn1 Al4 119.899(5) 3_565 2_665
Al4 Mn1 Al4 119.899(5) . 2_665
Al5 Mn1 Al3 75.90(5) . 5_566
Al5 Mn1 Al3 128.62(5) 3_565 5_566
Al5 Mn1 Al3 132.67(5) 2_665 5_566
Al4 Mn1 Al3 62.36(4) 3_565 5_566
Al4 Mn1 Al3 63.73(4) . 5_566
Al4 Mn1 Al3 149.33(6) 2_665 5_566
Al5 Mn1 Al3 132.67(5) . 4_666
Al5 Mn1 Al3 75.90(5) 3_565 4_666
Al5 Mn1 Al3 128.62(5) 2_665 4_666
Al4 Mn1 Al3 63.73(4) 3_565 4_666
Al4 Mn1 Al3 149.33(6) . 4_666
Al4 Mn1 Al3 62.36(4) 2_665 4_666
Al3 Mn1 Al3 98.71(5) 5_566 4_666
Al5 Mn1 Al3 128.62(5) . 6_556
Al5 Mn1 Al3 132.67(5) 3_565 6_556
Al5 Mn1 Al3 75.90(5) 2_665 6_556
Al4 Mn1 Al3 149.33(6) 3_565 6_556
Al4 Mn1 Al3 62.36(4) . 6_556
Al4 Mn1 Al3 63.73(4) 2_665 6_556
Al3 Mn1 Al3 98.71(5) 5_566 6_556
Al3 Mn1 Al3 98.71(5) 4_666 6_556
Al5 Mn1 Ge2 137.02(4) . .
Al5 Mn1 Ge2 137.02(4) 3_565 .
Al5 Mn1 Ge2 137.02(4) 2_665 .
Al4 Mn1 Ge2 88.17(4) 3_565 .
Al4 Mn1 Ge2 88.17(4) . .
Al4 Mn1 Ge2 88.17(4) 2_665 .
Al3 Mn1 Ge2 61.18(4) 5_566 .
Al3 Mn1 Ge2 61.18(4) 4_666 .
Al3 Mn1 Ge2 61.18(4) 6_556 .
Al9 Mn2 Al5 69.89(5) . 2_665
Al9 Mn2 Al7 125.45(5) . 6
Al5 Mn2 Al7 144.79(5) 2_665 6
Al9 Mn2 Al6 125.91(5) . 2_665
Al5 Mn2 Al6 74.48(5) 2_665 2_665
Al7 Mn2 Al6 71.47(5) 6 2_665
Al9 Mn2 Al6 67.91(5) . .
Al5 Mn2 Al6 80.99(5) 2_665 .
Al7 Mn2 Al6 78.00(5) 6 .
Al6 Mn2 Al6 67.39(6) 2_665 .
Al9 Mn2 Al8 73.33(5) . .
Al5 Mn2 Al8 68.16(5) 2_665 .
Al7 Mn2 Al8 142.80(5) 6 .
Al6 Mn2 Al8 127.20(5) 2_665 .
Al6 Mn2 Al8 136.80(5) . .
Al9 Mn2 Al6 127.07(5) . 5
Al5 Mn2 Al6 130.53(5) 2_665 5
Al7 Mn2 Al6 69.49(5) 6 5
Al6 Mn2 Al6 107.00(4) 2_665 5
Al6 Mn2 Al6 146.78(3) . 5
Al8 Mn2 Al6 73.90(5) . 5
Al9 Mn2 Al7 126.93(5) . 3_665
Al5 Mn2 Al7 67.05(5) 2_665 3_665
Al7 Mn2 Al7 107.61(4) 6 3_665
Al6 Mn2 Al7 68.87(4) 2_665 3_665
Al6 Mn2 Al7 131.06(5) . 3_665
Al8 Mn2 Al7 62.91(4) . 3_665
Al6 Mn2 Al7 67.97(4) 5 3_665
Al9 Mn2 Al2 66.07(5) . 6
Al5 Mn2 Al2 129.61(5) 2_665 6
Al7 Mn2 Al2 60.28(4) 6 6
Al6 Mn2 Al2 113.80(5) 2_665 6
Al6 Mn2 Al2 60.78(4) . 6
Al8 Mn2 Al2 118.63(5) . 6
Al6 Mn2 Al2 96.00(5) 5 6
Al7 Mn2 Al2 163.29(5) 3_665 6
Al9 Mn2 Al2 67.99(5) . .
Al5 Mn2 Al2 117.59(5) 2_665 .
Al7 Mn2 Al2 97.43(5) 6 .
Al6 Mn2 Al2 165.50(5) 2_665 .
Al6 Mn2 Al2 120.47(5) . .
Al8 Mn2 Al2 57.02(4) . .
Al6 Mn2 Al2 59.41(4) 5 .
Al7 Mn2 Al2 107.20(4) 3_665 .
Al2 Mn2 Al2 65.83(5) 6 .
Al9 Mn2 Mn2 178.49(5) . 4_665
Al5 Mn2 Mn2 109.59(5) 2_665 4_665
Al7 Mn2 Mn2 55.80(4) 6 4_665
Al6 Mn2 Mn2 54.91(4) 2_665 4_665
Al6 Mn2 Mn2 113.49(4) . 4_665
Al8 Mn2 Mn2 105.16(4) . 4_665
Al6 Mn2 Mn2 52.09(3) 5 4_665
Al7 Mn2 Mn2 51.80(4) 3_665 4_665
Al2 Mn2 Mn2 114.98(4) 6 4_665
Al2 Mn2 Mn2 111.30(4) . 4_665
Al9 Mn3 Al10 130.91(5) 3 .
Al9 Mn3 Al4 76.76(5) 3 3
Al10 Mn3 Al4 125.37(5) . 3
Al9 Mn3 Al8 126.89(5) 3 .
Al10 Mn3 Al8 67.46(5) . .
Al4 Mn3 Al8 139.70(5) 3 .
Al9 Mn3 Al3 118.86(5) 3 .
Al10 Mn3 Al3 109.90(5) . .
Al4 Mn3 Al3 61.90(5) 3 .
Al8 Mn3 Al3 77.80(5) . .
Al9 Mn3 Al7 70.88(5) 3 .
Al10 Mn3 Al7 140.66(5) . .
Al4 Mn3 Al7 88.31(5) 3 .
Al8 Mn3 Al7 73.55(5) . .
Al3 Mn3 Al7 65.27(5) . .
Al9 Mn3 Al10 122.79(5) 3 5_556
Al10 Mn3 Al10 60.72(5) . 5_556
Al4 Mn3 Al10 64.85(5) 3 5_556
Al8 Mn3 Al10 109.53(5) . 5_556
Al3 Mn3 Al10 78.52(5) . 5_556
Al7 Mn3 Al10 142.38(5) . 5_556
Al9 Mn3 Al10 66.05(5) 3 3
Al10 Mn3 Al10 86.12(6) . 3
Al4 Mn3 Al10 61.60(4) 3 3
Al8 Mn3 Al10 152.79(5) . 3
Al3 Mn3 Al10 119.30(5) . 3
Al7 Mn3 Al10 131.61(5) . 3
Al10 Mn3 Al10 58.92(4) 5_556 3
Al9 Mn3 Al2 68.75(5) 3 .
Al10 Mn3 Al2 94.46(5) . .
Al4 Mn3 Al2 139.00(5) 3 .
Al8 Mn3 Al2 59.62(4) . .
Al3 Mn3 Al2 117.38(5) . .
Al7 Mn3 Al2 60.22(4) . .
Al10 Mn3 Al2 154.78(5) 5_556 .
Al10 Mn3 Al2 119.11(5) 3 .
Al9 Mn3 Al1 70.20(5) 3 4
Al10 Mn3 Al1 60.76(4) . 4
Al4 Mn3 Al1 119.60(4) 3 4
Al8 Mn3 Al1 100.17(4) . 4
Al3 Mn3 Al1 170.09(6) . 4
Al7 Mn3 Al1 123.74(6) . 4
Al10 Mn3 Al1 93.22(6) 5_556 4
Al10 Mn3 Al1 59.12(4) 3 4
Al2 Mn3 Al1 68.60(5) . 4
Al1 Ge1 Al1 180.0 4 .
Al1 Ge1 Al2 70.91(3) 4 .
Al1 Ge1 Al2 109.09(3) . .
Al1 Ge1 Al2 109.09(3) 4 4
Al1 Ge1 Al2 70.91(3) . 4
Al2 Ge1 Al2 180.00(4) . 4
Al1 Ge1 Al2 109.09(3) 4 5
Al1 Ge1 Al2 70.91(3) . 5
Al2 Ge1 Al2 70.15(3) . 5
Al2 Ge1 Al2 109.85(3) 4 5
Al1 Ge1 Al2 109.09(3) 4 6
Al1 Ge1 Al2 70.91(3) . 6
Al2 Ge1 Al2 70.15(3) . 6
Al2 Ge1 Al2 109.85(3) 4 6
Al2 Ge1 Al2 109.85(3) 5 6
Al1 Ge1 Al2 70.91(3) 4 2
Al1 Ge1 Al2 109.09(3) . 2
Al2 Ge1 Al2 109.85(3) . 2
Al2 Ge1 Al2 70.15(3) 4 2
Al2 Ge1 Al2 180.00(4) 5 2
Al2 Ge1 Al2 70.15(3) 6 2
Al1 Ge1 Al2 70.91(3) 4 3
Al1 Ge1 Al2 109.09(3) . 3
Al2 Ge1 Al2 109.85(3) . 3
Al2 Ge1 Al2 70.15(3) 4 3
Al2 Ge1 Al2 70.15(3) 5 3
Al2 Ge1 Al2 180.0 6 3
Al2 Ge1 Al2 109.85(3) 2 3
Al8 Ge2 Al8 119.843(5) 5_566 6_556
Al8 Ge2 Al8 119.843(5) 5_566 4_666
Al8 Ge2 Al8 119.843(5) 6_556 4_666
Al8 Ge2 Al3 71.91(4) 5_566 5_566
Al8 Ge2 Al3 63.54(4) 6_556 5_566
Al8 Ge2 Al3 145.73(5) 4_666 5_566
Al8 Ge2 Al3 63.54(4) 5_566 4_666
Al8 Ge2 Al3 145.73(5) 6_556 4_666
Al8 Ge2 Al3 71.91(4) 4_666 4_666
Al3 Ge2 Al3 88.72(5) 5_566 4_666
Al8 Ge2 Al3 145.73(5) 5_566 6_556
Al8 Ge2 Al3 71.91(4) 6_556 6_556
Al8 Ge2 Al3 63.54(4) 4_666 6_556
Al3 Ge2 Al3 88.72(5) 5_566 6_556
Al3 Ge2 Al3 88.72(5) 4_666 6_556
Al8 Ge2 Mn1 92.28(3) 5_566 .
Al8 Ge2 Mn1 92.28(3) 6_556 .
Al8 Ge2 Mn1 92.28(3) 4_666 .
Al3 Ge2 Mn1 53.84(3) 5_566 .
Al3 Ge2 Mn1 53.84(3) 4_666 .
Al3 Ge2 Mn1 53.84(3) 6_556 .
Ge1 Al1 Al10 130.49(5) . 4
Ge1 Al1 Al10 130.49(5) . 5
Al10 Al1 Al10 82.39(7) 4 5
Ge1 Al1 Al10 130.49(5) . 6
Al10 Al1 Al10 82.39(7) 4 6
Al10 Al1 Al10 82.39(7) 5 6
Ge1 Al1 Mn3 106.70(5) . 4
Al10 Al1 Mn3 54.80(4) 4 4
Al10 Al1 Mn3 122.77(9) 5 4
Al10 Al1 Mn3 58.36(4) 6 4
Ge1 Al1 Mn3 106.70(5) . 6
Al10 Al1 Mn3 122.77(9) 4 6
Al10 Al1 Mn3 58.36(4) 5 6
Al10 Al1 Mn3 54.80(4) 6 6
Mn3 Al1 Mn3 112.10(4) 4 6
Ge1 Al1 Mn3 106.70(5) . 5
Al10 Al1 Mn3 58.36(4) 4 5
Al10 Al1 Mn3 54.80(4) 5 5
Al10 Al1 Mn3 122.77(9) 6 5
Mn3 Al1 Mn3 112.10(4) 4 5
Mn3 Al1 Mn3 112.10(4) 6 5
Ge1 Al1 Al9 76.54(5) . 5
Al10 Al1 Al9 138.03(6) 4 5
Al10 Al1 Al9 58.08(4) 5 5
Al10 Al1 Al9 103.80(5) 6 5
Mn3 Al1 Al9 159.61(3) 4 5
Mn3 Al1 Al9 49.04(3) 6 5
Mn3 Al1 Al9 85.35(3) 5 5
Ge1 Al1 Al9 76.54(5) . 4
Al10 Al1 Al9 58.08(4) 4 4
Al10 Al1 Al9 103.80(5) 5 4
Al10 Al1 Al9 138.03(6) 6 4
Mn3 Al1 Al9 85.35(3) 4 4
Mn3 Al1 Al9 159.61(3) 6 4
Mn3 Al1 Al9 49.04(3) 5 4
Al9 Al1 Al9 114.75(4) 5 4
Ge1 Al1 Al9 76.54(5) . 6
Al10 Al1 Al9 103.80(5) 4 6
Al10 Al1 Al9 138.03(6) 5 6
Al10 Al1 Al9 58.08(4) 6 6
Mn3 Al1 Al9 49.04(3) 4 6
Mn3 Al1 Al9 85.35(3) 6 6
Mn3 Al1 Al9 159.61(3) 5 6
Al9 Al1 Al9 114.75(4) 5 6
Al9 Al1 Al9 114.75(4) 4 6
Al8 Al2 Ge1 137.83(6) . .
Al8 Al2 Al7 71.69(5) . .
Ge1 Al2 Al7 137.80(6) . .
Al8 Al2 Mn3 57.41(4) . .
Ge1 Al2 Mn3 107.15(5) . .
Al7 Al2 Mn3 58.25(4) . .
Al8 Al2 Al6 72.10(5) . 5
Ge1 Al2 Al6 135.43(6) . 5
Al7 Al2 Al6 73.30(5) . 5
Mn3 Al2 Al6 117.39(6) . 5
Al8 Al2 Mn2 112.53(6) . 5
Ge1 Al2 Mn2 109.63(5) . 5
Al7 Al2 Mn2 55.11(4) . 5
Mn3 Al2 Mn2 111.08(5) . 5
Al6 Al2 Mn2 56.21(4) 5 5
Al8 Al2 Al9 130.29(7) . 5
Ge1 Al2 Al9 78.29(5) . 5
Al7 Al2 Al9 105.04(6) . 5
Mn3 Al2 Al9 160.74(6) . 5
Al6 Al2 Al9 60.22(5) 5 5
Mn2 Al2 Al9 50.54(4) 5 5
Al8 Al2 Mn2 56.77(4) . .
Ge1 Al2 Mn2 107.31(5) . .
Al7 Al2 Mn2 114.89(6) . .
Mn3 Al2 Mn2 111.05(5) . .
Al6 Al2 Mn2 55.91(4) 5 .
Mn2 Al2 Mn2 110.48(5) 5 .
Al9 Al2 Mn2 83.92(5) 5 .
Al8 Al2 Al9 106.70(6) . 3
Ge1 Al2 Al9 77.53(4) . 3
Al7 Al2 Al9 62.90(5) . 3
Mn3 Al2 Al9 50.28(4) . 3
Al6 Al2 Al9 133.26(6) 5 3
Mn2 Al2 Al9 84.55(5) 5 3
Al9 Al2 Al9 115.53(6) 5 3
Mn2 Al2 Al9 160.53(6) . 3
Al8 Al2 Al9 64.60(5) . .
Ge1 Al2 Al9 76.13(4) . .
Al7 Al2 Al9 134.21(6) . .
Mn3 Al2 Al9 86.19(5) . .
Al6 Al2 Al9 104.34(6) 5 .
Mn2 Al2 Al9 158.04(6) 5 .
Al9 Al2 Al9 113.05(6) 5 .
Mn2 Al2 Al9 48.64(4) . .
Al9 Al2 Al9 117.36(7) 3 .
Mn1 Al3 Mn3 130.87(6) 4_666 .
Mn1 Al3 Al4 58.66(4) 4_666 5_556
Mn3 Al3 Al4 75.46(5) . 5_556
Mn1 Al3 Al4 147.23(7) 4_666 3
Mn3 Al3 Al4 58.28(4) . 3
Al4 Al3 Al4 106.09(7) 5_556 3
Mn1 Al3 Al4 57.97(4) 4_666 6_656
Mn3 Al3 Al4 170.61(7) . 6_656
Al4 Al3 Al4 111.44(8) 5_556 6_656
Al4 Al3 Al4 112.77(6) 3 6_656
Mn1 Al3 Ge2 64.99(4) 4_666 4_666
Mn3 Al3 Ge2 99.48(5) . 4_666
Al4 Al3 Ge2 88.35(5) 5_556 4_666
Al4 Al3 Ge2 147.50(6) 3 4_666
Al4 Al3 Ge2 87.31(5) 6_656 4_666
Mn1 Al3 Al7 129.82(6) 4_666 .
Mn3 Al3 Al7 58.18(4) . .
Al4 Al3 Al7 118.70(6) 5_556 .
Al4 Al3 Al7 82.76(6) 3 .
Al4 Al3 Al7 120.31(6) 6_656 .
Ge2 Al3 Al7 64.85(4) 4_666 .
Mn1 Al3 Al8 95.58(5) 4_666 2_655
Mn3 Al3 Al8 115.64(6) . 2_655
Al4 Al3 Al8 145.15(7) 5_556 2_655
Al4 Al3 Al8 107.54(6) 3 2_655
Al4 Al3 Al8 62.62(5) 6_656 2_655
Ge2 Al3 Al8 57.95(4) 4_666 2_655
Al7 Al3 Al8 57.80(5) . 2_655
Mn1 Al3 Al3 105.59(7) 4_666 4_656
Mn3 Al3 Al3 115.40(7) . 4_656
Al4 Al3 Al3 125.53(8) 5_556 4_656
Al4 Al3 Al3 57.20(5) 3 4_656
Al4 Al3 Al3 55.58(5) 6_656 4_656
Ge2 Al3 Al3 135.38(7) 4_666 4_656
Al7 Al3 Al3 110.32(7) . 4_656
Al8 Al3 Al3 81.40(6) 2_655 4_656
Mn1 Al4 Mn3 147.52(7) . 2
Mn1 Al4 Al3 58.98(4) . 6_556
Mn3 Al4 Al3 138.52(7) 2 6_556
Mn1 Al4 Al3 115.74(6) . 2
Mn3 Al4 Al3 59.82(4) 2 2
Al3 Al4 Al3 155.95(6) 6_556 2
Mn1 Al4 Al10 125.54(6) . .
Mn3 Al4 Al10 61.25(4) 2 .
Al3 Al4 Al10 77.31(6) 6_556 .
Al3 Al4 Al10 117.07(6) 2 .
Mn1 Al4 Al3 58.29(4) . 5_566
Mn3 Al4 Al3 126.96(6) 2 5_566
Al3 Al4 Al3 93.24(7) 6_556 5_566
Al3 Al4 Al3 67.23(6) 2 5_566
Al10 Al4 Al3 161.77(7) . 5_566
Mn1 Al4 Al10 153.13(7) . 6_556
Mn3 Al4 Al10 59.33(4) 2 6_556
Al3 Al4 Al10 100.52(6) 6_556 6_556
Al3 Al4 Al10 75.21(5) 2 6_556
Al10 Al4 Al10 57.13(6) . 6_556
Al3 Al4 Al10 110.62(6) 5_566 6_556
Mn1 Al4 Al5 53.33(4) . .
Mn3 Al4 Al5 96.82(6) 2 .
Al3 Al4 Al5 109.68(6) 6_556 .
Al3 Al4 Al5 76.53(5) 2 .
Al10 Al4 Al5 130.67(7) . .
Al3 Al4 Al5 67.07(5) 5_566 .
Al10 Al4 Al5 149.76(7) 6_556 .
Mn1 Al4 Al8 95.60(6) . 6_556
Mn3 Al4 Al8 115.34(6) 2 6_556
Al3 Al4 Al8 71.25(5) 6_556 6_556
Al3 Al4 Al8 86.76(6) 2 6_556
Al10 Al4 Al8 99.62(6) . 6_556
Al3 Al4 Al8 62.35(5) 5_566 6_556
Al10 Al4 Al8 59.32(5) 6_556 6_556
Al5 Al4 Al8 129.33(6) . 6_556
Mn1 Al4 Al5 52.05(4) . 2_665
Mn3 Al4 Al5 104.40(6) 2 2_665
Al3 Al4 Al5 66.28(5) 6_556 2_665
Al3 Al4 Al5 131.63(7) 2 2_665
Al10 Al4 Al5 82.66(5) . 2_665
Al3 Al4 Al5 108.03(6) 5_566 2_665
Al10 Al4 Al5 139.77(6) 6_556 2_665
Al5 Al4 Al5 59.33(6) . 2_665
Al8 Al4 Al5 135.85(6) 6_556 2_665
Mn1 Al5 Mn2 162.87(7) . 3_565
Mn1 Al5 Al9 115.96(6) . 3_565
Mn2 Al5 Al9 54.37(4) 3_565 3_565
Mn1 Al5 Al7 134.47(6) . 2
Mn2 Al5 Al7 60.13(4) 3_565 2
Al9 Al5 Al7 107.99(6) 3_565 2
Mn1 Al5 Al8 133.40(7) . 3_565
Mn2 Al5 Al8 58.81(4) 3_565 3_565
Al9 Al5 Al8 64.63(5) 3_565 3_565
Al7 Al5 Al8 58.18(5) 2 3_565
Mn1 Al5 Al4 56.51(4) . .
Mn2 Al5 Al4 138.48(7) 3_565 .
Al9 Al5 Al4 156.27(7) 3_565 .
Al7 Al5 Al4 78.46(5) 2 .
Al8 Al5 Al4 103.00(6) 3_565 .
Mn1 Al5 Al5 53.82(3) . 3_565
Mn2 Al5 Al5 109.05(5) 3_565 3_565
Al9 Al5 Al5 79.04(7) 3_565 3_565
Al7 Al5 Al5 151.97(5) 2 3_565
Al8 Al5 Al5 141.89(8) 3_565 3_565
Al4 Al5 Al5 106.28(5) . 3_565
Mn1 Al5 Al5 53.82(3) . 2_665
Mn2 Al5 Al5 120.63(4) 3_565 2_665
Al9 Al5 Al5 135.15(7) 3_565 2_665
Al7 Al5 Al5 101.40(7) 2 2_665
Al8 Al5 Al5 158.08(8) 3_565 2_665
Al4 Al5 Al5 61.98(5) . 2_665
Al5 Al5 Al5 60.0 3_565 2_665
Mn1 Al5 Al4 55.09(4) . 3_565
Mn2 Al5 Al4 118.69(6) 3_565 3_565
Al9 Al5 Al4 64.42(5) 3_565 3_565
Al7 Al5 Al4 149.13(7) 2 3_565
Al8 Al5 Al4 93.68(6) 3_565 3_565
Al4 Al5 Al4 98.02(7) . 3_565
Al5 Al5 Al4 58.69(5) 3_565 3_565
Al5 Al5 Al4 103.82(5) 2_665 3_565
Mn2 Al6 Mn2 152.38(6) 3_565 .
Mn2 Al6 Mn2 73.00(4) 3_565 6
Mn2 Al6 Mn2 125.46(6) . 6
Mn2 Al6 Al2 137.33(6) 3_565 6
Mn2 Al6 Al2 63.01(4) . 6
Mn2 Al6 Al2 64.68(4) 6 6
Mn2 Al6 Al9 114.07(6) 3_565 .
Mn2 Al6 Al9 52.77(4) . .
Mn2 Al6 Al9 89.47(5) 6 .
Al2 Al6 Al9 62.01(5) 6 .
Mn2 Al6 Al6 115.69(5) 3_565 2_665
Mn2 Al6 Al6 55.18(5) . 2_665
Mn2 Al6 Al6 159.63(3) 6 2_665
Al2 Al6 Al6 106.13(7) 6 2_665
Al9 Al6 Al6 102.31(6) . 2_665
Mn2 Al6 Al6 57.43(5) 3_565 3_565
Mn2 Al6 Al6 113.51(5) . 3_565
Mn2 Al6 Al6 120.24(7) 6 3_565
Al2 Al6 Al6 154.50(5) 6 3_565
Al9 Al6 Al6 138.40(4) . 3_565
Al6 Al6 Al6 60.0 2_665 3_565
Mn2 Al6 Al7 57.67(4) 3_565 2
Mn2 Al6 Al7 113.52(6) . 2
Mn2 Al6 Al7 53.73(4) 6 2
Al2 Al6 Al7 91.43(5) 6 2
Al9 Al6 Al7 60.92(5) . 2
Al6 Al6 Al7 146.64(4) 2_665 2
Al6 Al6 Al7 111.71(6) 3_565 2
Mn2 Al6 Al7 54.24(4) 3_565 5_565
Mn2 Al6 Al7 151.32(6) . 5_565
Mn2 Al6 Al7 56.62(4) 6 5_565
Al2 Al6 Al7 103.00(6) 6 5_565
Al9 Al6 Al7 145.52(6) . 5_565
Al6 Al6 Al7 111.92(5) 2_665 5_565
Al6 Al6 Al7 67.57(5) 3_565 5_565
Al7 Al6 Al7 90.63(5) 2 5_565
Mn2 Al7 Mn3 123.20(6) 5 .
Mn2 Al7 Mn2 72.39(4) 5 2_655
Mn3 Al7 Mn2 147.10(6) . 2_655
Mn2 Al7 Al2 64.61(4) 5 .
Mn3 Al7 Al2 61.52(4) . .
Mn2 Al7 Al2 135.28(6) 2_655 .
Mn2 Al7 Al8 117.69(6) 5 2_655
Mn3 Al7 Al8 118.95(6) . 2_655
Mn2 Al7 Al8 57.78(4) 2_655 2_655
Al2 Al7 Al8 158.07(7) . 2_655
Mn2 Al7 Al3 170.10(7) 5 .
Mn3 Al7 Al3 56.55(4) . .
Mn2 Al7 Al3 113.37(6) 2_655 .
Al2 Al7 Al3 111.00(6) . .
Al8 Al7 Al3 62.75(5) 2_655 .
Mn2 Al7 Al5 114.97(6) 5 3
Mn3 Al7 Al5 95.53(5) . 3
Mn2 Al7 Al5 52.82(4) 2_655 3
Al2 Al7 Al5 139.73(7) . 3
Al8 Al7 Al5 61.18(5) 2_655 3
Al3 Al7 Al5 74.32(5) . 3
Mn2 Al7 Al9 88.89(5) 5 3
Mn3 Al7 Al9 50.75(4) . 3
Mn2 Al7 Al9 106.72(5) 2_655 3
Al2 Al7 Al9 62.13(5) . 3
Al8 Al7 Al9 137.22(6) 2_655 3
Al3 Al7 Al9 96.76(5) . 3
Al5 Al7 Al9 77.67(5) 3 3
Mn2 Al7 Al6 56.78(4) 5 3
Mn3 Al7 Al6 107.67(6) . 3
Mn2 Al7 Al6 53.45(4) 2_655 3
Al2 Al7 Al6 91.35(6) . 3
Al8 Al7 Al6 108.16(6) 2_655 3
Al3 Al7 Al6 133.08(6) . 3
Al5 Al7 Al6 62.97(5) 3 3
Al9 Al7 Al6 57.18(4) 3 3
Mn2 Al7 Al6 54.29(4) 5 6_655
Mn3 Al7 Al6 157.40(6) . 6_655
Mn2 Al7 Al6 55.42(4) 2_655 6_655
Al2 Al7 Al6 104.45(6) . 6_655
Al8 Al7 Al6 66.89(5) 2_655 6_655
Al3 Al7 Al6 121.42(6) . 6_655
Al5 Al7 Al6 105.59(6) 3 6_655
Al9 Al7 Al6 141.40(6) 3 6_655
Al6 Al7 Al6 89.37(5) 3 6_655
Mn3 Al8 Mn2 125.00(5) . .
Mn3 Al8 Al2 62.98(5) . .
Mn2 Al8 Al2 66.21(5) . .
Mn3 Al8 Ge2 100.20(5) . 4_666
Mn2 Al8 Ge2 115.67(5) . 4_666
Al2 Al8 Ge2 109.72(6) . 4_666
Mn3 Al8 Al7 163.12(6) . 3_665
Mn2 Al8 Al7 59.31(4) . 3_665
Al2 Al8 Al7 111.53(6) . 3_665
Ge2 Al8 Al7 65.72(4) 4_666 3_665
Mn3 Al8 Al10 55.13(4) . .
Mn2 Al8 Al10 105.93(5) . .
Al2 Al8 Al10 89.40(6) . .
Ge2 Al8 Al10 138.27(6) 4_666 .
Al7 Al8 Al10 141.67(6) 3_665 .
Mn3 Al8 Al5 136.03(6) . 2_665
Mn2 Al8 Al5 53.03(4) . 2_665
Al2 Al8 Al5 112.49(6) . 2_665
Ge2 Al8 Al5 120.35(5) 4_666 2_665
Al7 Al8 Al5 60.65(5) 3_665 2_665
Al10 Al8 Al5 81.99(5) . 2_665
Mn3 Al8 Al3 122.47(6) . 3_665
Mn2 Al8 Al3 111.81(5) . 3_665
Al2 Al8 Al3 166.75(7) . 3_665
Ge2 Al8 Al3 58.51(4) 4_666 3_665
Al7 Al8 Al3 59.45(5) 3_665 3_665
Al10 Al8 Al3 103.56(6) . 3_665
Al5 Al8 Al3 72.73(5) 2_665 3_665
Mn3 Al8 Al4 70.94(4) . 5_556
Mn2 Al8 Al4 148.51(6) . 5_556
Al2 Al8 Al4 133.52(6) . 5_556
Ge2 Al8 Al4 83.32(5) 4_666 5_556
Al7 Al8 Al4 114.39(6) 3_665 5_556
Al10 Al8 Al4 58.06(5) . 5_556
Al5 Al8 Al4 96.05(6) 2_665 5_556
Al3 Al8 Al4 55.03(5) 3_665 5_556
Mn3 Al8 Al9 88.15(5) . .
Mn2 Al8 Al9 50.07(4) . .
Al2 Al8 Al9 63.27(5) . .
Ge2 Al8 Al9 165.27(6) 4_666 .
Al7 Al8 Al9 103.77(6) 3_665 .
Al10 Al8 Al9 56.34(4) . .
Al5 Al8 Al9 56.68(5) 2_665 .
Al3 Al8 Al9 126.48(6) 3_665 .
Al4 Al8 Al9 111.02(6) 5_556 .
Mn3 Al9 Mn2 169.96(7) 2 .
Mn3 Al9 Al10 61.51(4) 2 .
Mn2 Al9 Al10 114.32(6) . .
Mn3 Al9 Al5 114.22(6) 2 2_665
Mn2 Al9 Al5 55.74(4) . 2_665
Al10 Al9 Al5 84.23(6) . 2_665
Mn3 Al9 Al6 119.95(6) 2 .
Mn2 Al9 Al6 59.32(4) . .
Al10 Al9 Al6 154.45(7) . .
Al5 Al9 Al6 71.97(5) 2_665 .
Mn3 Al9 Al2 125.65(6) 2 6
Mn2 Al9 Al2 63.39(4) . 6
Al10 Al9 Al2 145.15(7) . 6
Al5 Al9 Al2 114.63(6) 2_665 6
Al6 Al9 Al2 57.77(5) . 6
Mn3 Al9 Al2 60.96(4) 2 2
Mn2 Al9 Al2 127.96(6) . 2
Al10 Al9 Al2 109.88(6) . 2
Al5 Al9 Al2 156.00(7) 2_665 2
Al6 Al9 Al2 89.94(5) . 2
Al2 Al9 Al2 64.70(5) 6 2
Mn3 Al9 Al7 58.37(4) 2 2
Mn2 Al9 Al7 121.01(6) . 2
Al10 Al9 Al7 116.14(6) . 2
Al5 Al9 Al7 101.67(6) 2_665 2
Al6 Al9 Al7 61.90(5) . 2
Al2 Al9 Al7 89.63(5) 6 2
Al2 Al9 Al7 54.97(4) 2 2
Mn3 Al9 Al2 123.11(6) 2 .
Mn2 Al9 Al2 63.37(4) . .
Al10 Al9 Al2 83.86(5) . .
Al5 Al9 Al2 104.48(6) 2_665 .
Al6 Al9 Al2 110.55(6) . .
Al2 Al9 Al2 63.66(5) 6 .
Al2 Al9 Al2 96.48(7) 2 .
Al7 Al9 Al2 148.53(6) 2 .
Mn3 Al9 Al1 60.76(4) 2 4
Mn2 Al9 Al1 125.63(6) . 4
Al10 Al9 Al1 55.38(6) . 4
Al5 Al9 Al1 137.47(7) 2_665 4
Al6 Al9 Al1 149.87(7) . 4
Al2 Al9 Al1 96.05(7) 6 4
Al2 Al9 Al1 63.40(5) 2 4
Al7 Al9 Al1 107.51(5) 2 4
Al2 Al9 Al1 62.46(5) . 4
Mn3 Al9 Al8 119.77(6) 2 .
Mn2 Al9 Al8 56.60(4) . .
Al10 Al9 Al8 58.28(5) . .
Al5 Al9 Al8 58.69(5) 2_665 .
Al6 Al9 Al8 113.32(6) . .
Al2 Al9 Al8 105.13(6) 6 .
Al2 Al9 Al8 145.22(6) 2 .
Al7 Al9 Al8 158.92(6) 2 .
Al2 Al9 Al8 52.14(4) . .
Al1 Al9 Al8 86.18(5) 4 .
Mn3 Al10 Al10 62.27(4) . 5_556
Mn3 Al10 Al10 137.97(4) . 6_556
Al10 Al10 Al10 85.10(7) 5_556 6_556
Mn3 Al10 Mn3 117.34(5) . 6_556
Al10 Al10 Mn3 60.72(6) 5_556 6_556
Al10 Al10 Mn3 57.00(6) 6_556 6_556
Mn3 Al10 Mn3 125.55(6) . 2
Al10 Al10 Mn3 134.53(4) 5_556 2
Al10 Al10 Mn3 60.35(4) 6_556 2
Mn3 Al10 Mn3 112.28(5) 6_556 2
Mn3 Al10 Al4 158.15(7) . .
Al10 Al10 Al4 134.24(8) 5_556 .
Al10 Al10 Al4 63.76(5) 6_556 .
Mn3 Al10 Al4 74.01(5) 6_556 .
Mn3 Al10 Al4 57.15(4) 2 .
Mn3 Al10 Al1 64.43(4) . 4
Al10 Al10 Al1 96.24(4) 5_556 4
Al10 Al10 Al1 96.24(4) 6_556 4
Mn3 Al10 Al1 143.82(7) 6_556 4
Mn3 Al10 Al1 62.52(3) 2 4
Al4 Al10 Al1 118.58(6) . 4
Mn3 Al10 Al9 95.44(5) . .
Al10 Al10 Al9 156.88(7) 5_556 .
Al10 Al10 Al9 111.07(6) 6_556 .
Mn3 Al10 Al9 141.85(6) 6_556 .
Mn3 Al10 Al9 52.43(4) 2 .
Al4 Al10 Al9 68.87(5) . .
Al1 Al10 Al9 66.54(6) 4 .
Mn3 Al10 Al4 74.11(5) . 5_556
Al10 Al10 Al4 59.12(6) 5_556 5_556
Al10 Al10 Al4 112.65(8) 6_556 5_556
Mn3 Al10 Al4 55.81(4) 6_556 5_556
Mn3 Al10 Al4 158.49(6) 2 5_556
Al4 Al10 Al4 101.34(5) . 5_556
Al1 Al10 Al4 138.34(6) 4 5_556
Al9 Al10 Al4 123.60(6) . 5_556
Mn3 Al10 Al8 57.41(4) . .
Al10 Al10 Al8 103.44(6) 5_556 .
Al10 Al10 Al8 163.90(6) 6_556 .
Mn3 Al10 Al8 115.13(6) 6_556 .
Mn3 Al10 Al8 117.79(6) 2 .
Al4 Al10 Al8 101.24(6) . .
Al1 Al10 Al8 96.35(6) 4 .
Al9 Al10 Al8 65.38(5) . .
Al4 Al10 Al8 62.61(5) 5_556 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mn1 Al5 2.4307(16) .
Mn1 Al5 2.4307(16) 3_565
Mn1 Al5 2.4307(16) 2_665
Mn1 Al4 2.5276(14) 3_565
Mn1 Al4 2.5276(14) .
Mn1 Al4 2.5276(14) 2_665
Mn1 Al3 2.5363(15) 5_566
Mn1 Al3 2.5363(15) 4_666
Mn1 Al3 2.5363(15) 6_556
Mn1 Ge2 2.8469(15) .
Mn2 Al9 2.4007(15) .
Mn2 Al5 2.4411(15) 2_665
Mn2 Al7 2.5245(15) 6
Mn2 Al6 2.5260(15) 2_665
Mn2 Al6 2.5930(15) .
Mn2 Al8 2.6137(15) .
Mn2 Al6 2.6196(15) 5
Mn2 Al7 2.6569(15) 3_665
Mn2 Al2 2.7802(15) 6
Mn2 Al2 2.8592(16) .
Mn2 Mn2 3.0616(13) 4_665
Mn3 Al9 2.3814(15) 3
Mn3 Al10 2.4929(15) .
Mn3 Al4 2.5302(15) 3
Mn3 Al8 2.5599(15) .
Mn3 Al3 2.5714(15) .
Mn3 Al7 2.6186(15) .
Mn3 Al10 2.6310(15) 5_556
Mn3 Al10 2.6406(15) 3
Mn3 Al2 2.7067(15) .
Mn3 Al1 2.7519(10) 4
Ge1 Al1 2.637(2) 4
Ge1 Al1 2.637(2) .
Ge1 Al2 2.6666(14) .
Ge1 Al2 2.6666(14) 4
Ge1 Al2 2.6666(14) 5
Ge1 Al2 2.6666(14) 6
Ge1 Al2 2.6666(14) 2
Ge1 Al2 2.6666(14) 3
Ge2 Al8 2.7359(14) 5_566
Ge2 Al8 2.7359(14) 6_556
Ge2 Al8 2.7359(14) 4_666
Ge2 Al3 2.7524(15) 5_566
Ge2 Al3 2.7524(15) 4_666
Ge2 Al3 2.7524(15) 6_556
Al1 Al10 2.662(2) 4
Al1 Al10 2.662(2) 5
Al1 Al10 2.662(2) 6
Al1 Mn3 2.7519(10) 4
Al1 Mn3 2.7519(10) 6
Al1 Mn3 2.7519(10) 5
Al1 Al9 2.9673(16) 5
Al1 Al9 2.9673(16) 4
Al1 Al9 2.9673(16) 6
Al2 Al8 2.6212(19) .
Al2 Al7 2.6727(19) .
Al2 Al6 2.7228(19) 5
Al2 Mn2 2.7802(15) 5
Al2 Al9 2.842(2) 5
Al2 Al9 2.885(2) 3
Al2 Al9 2.965(2) .
Al3 Mn1 2.5363(15) 4_666
Al3 Al4 2.6218(19) 5_556
Al3 Al4 2.624(2) 3
Al3 Al4 2.6735(19) 6_656
Al3 Ge2 2.7524(15) 4_666
Al3 Al7 2.7992(19) .
Al3 Al8 2.8898(19) 2_655
Al3 Al3 2.933(3) 4_656
Al4 Mn3 2.5302(15) 2
Al4 Al3 2.622(2) 6_556
Al4 Al3 2.624(2) 2
Al4 Al10 2.6494(19) .
Al4 Al3 2.6735(19) 5_566
Al4 Al10 2.7689(19) 6_556
Al4 Al5 2.851(2) .
Al4 Al8 2.897(2) 6_556
Al4 Al5 2.946(2) 2_665
Al5 Mn2 2.4411(15) 3_565
Al5 Al9 2.774(2) 3_565
Al5 Al7 2.821(2) 2
Al5 Al8 2.836(2) 3_565
Al5 Al5 2.870(2) 3_565
Al5 Al5 2.870(2) 2_665
Al5 Al4 2.946(2) 3_565
Al6 Mn2 2.5260(15) 3_565
Al6 Mn2 2.6196(15) 6
Al6 Al2 2.7228(19) 6
Al6 Al9 2.7939(19) .
Al6 Al6 2.840(2) 2_665
Al6 Al6 2.840(2) 3_565
Al6 Al7 2.9328(19) 2
Al6 Al7 2.9495(19) 5_565
Al7 Mn2 2.5245(15) 5
Al7 Mn2 2.6569(15) 2_655
Al7 Al8 2.7504(19) 2_655
Al7 Al5 2.821(2) 3
Al7 Al9 2.906(2) 3
Al7 Al6 2.9328(19) 3
Al7 Al6 2.9495(19) 6_655
Al8 Ge2 2.7359(14) 4_666
Al8 Al7 2.7504(19) 3_665
Al8 Al10 2.8062(19) .
Al8 Al5 2.836(2) 2_665
Al8 Al3 2.8898(19) 3_665
Al8 Al4 2.897(2) 5_556
Al8 Al9 2.9992(19) .
Al9 Mn3 2.3814(15) 2
Al9 Al10 2.7458(19) .
Al9 Al5 2.774(2) 2_665
Al9 Al2 2.842(2) 6
Al9 Al2 2.885(2) 2
Al9 Al7 2.906(2) 2
Al9 Al1 2.9673(16) 4
Al10 Al10 2.593(2) 5_556
Al10 Al10 2.593(2) 6_556
Al10 Mn3 2.6310(15) 6_556
Al10 Mn3 2.6406(15) 2
Al10 Al1 2.662(2) 4
Al10 Al4 2.7689(19) 5_556
